LMucko/crystallography-open-database huggingface dataset:
Oxidation of hexasilver to silver chloride by dichlorine. Crystal structure of H2.25 Ag12 Cl2.25 Si12 Al12 O48 * (Cl2)6 a chlorine sorption complex of partially dehydrated fully Ag+ -exchanged ...
Kim, Y.; Seff, K.; Journal of the American Chemical Society 100 (1978) 3801–3805; doi:

data_4124443
_publ_section_title
;
 Oxidation of hexasilver to silver chloride by dichlorine. Crystal
 structure of H2.25 Ag12 Cl2.25 Si12 Al12 O48 * (Cl2)6 a chlorine sorption
 complex of partially dehydrated fully Ag+ -exchanged ...
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              3801
_journal_page_last               3805
_journal_volume                  100
_journal_year                    1978
_chemical_formula_sum            'Ag12 Al12 Cl14.248 H2.25 O48 Si12'
_chemical_name_systematic        'H2.25 Ag12 Cl2.248 Si12 Al12 O48 (Cl2)6'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   12.244
_cell_length_b                   12.244
_cell_length_c                   12.244
_cell_volume                     1835.566
_citation_journal_id_ASTM        JACSAT
_cod_data_source_file            Kim_JACSAT_1978_285.cif
_cod_data_source_block           H2.25Ag12Al12Cl14.248O48Si12
_cod_original_formula_sum        'H2.25 Ag12 Al12 Cl14.248 O48 Si12'
_cod_database_code               4124443
The octahedral hexasilver molecule. Seven crystal structures of variously vacuum-dehydrated fully Ag+ -exchanged zeolite A
Kim, Y.; Seff, K.; Journal of the American Chemical Society 100 (1978) 6989–6997; doi:

data_4124444
_publ_section_title
;
 The octahedral hexasilver molecule. Seven crystal structures of variously
 vacuum-dehydrated fully Ag+ -exchanged zeolite A
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              6989
_journal_page_last               6997
_journal_volume                  100
_journal_year                    1978
_chemical_formula_sum            'Ag7.48 Al12 O48 Si12'
_chemical_name_systematic        'Ag7.48 Si12 Al12 O48'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   12.279
_cell_length_b                   12.279
_cell_length_c                   12.279
_cell_volume                     1851.352
_citation_journal_id_ASTM        JACSAT
_cod_data_source_file            Kim_JACSAT_1978_288.cif
_cod_data_source_block           Ag7.48Al12O48Si12
_cod_database_code               4124444
On the Stabilization of Zr5 Al3 in the Mn5 Si3-type structure by Interstitial Oxygen
Kim, S.-J.; Yi, S.S.; Kematick, R.J.; Franzen, H.F.; Journal of the Less-Common Metals 137 (1988) 55–59; doi:

data_1530163
_publ_section_title
;
 On the Stabilization of Zr5 Al3 in the Mn5 Si3-type structure by
 Interstitial Oxygen
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              55
_journal_page_last               59
_journal_volume                  137
_journal_year                    1988
_chemical_formula_sum            'Al3 O0.34 Zr5'
_chemical_name_systematic        'Zr5 Al3 O.34'
_space_group_IT_number           193
_symmetry_space_group_name_Hall  '-P 6c 2'
_symmetry_space_group_name_H-M   'P 63/m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   8.248
_cell_length_b                   8.248
_cell_length_c                   5.706
_cell_volume                     336.171
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            Kim_JCOMAH_1988_1592.cif
_cod_data_source_block           Al3O0.34Zr5
_cod_original_cell_volume        336.1706
_cod_database_code               1530163
Cation and Oxygen Disorder in the Structures Tl Sr2 Cu O5 And (Pb.63 Cu.37) Sr2 Co O5
Kim, J.S.; Swinnea, J.S.; Steinfink, H.; Journal of the Less-Common Metals 156 (1989) 347–355; doi:

data_1530164
_publ_section_title
;
 Cation and Oxygen Disorder in the Structures Tl Sr2 Cu O5 And (Pb.63
 Cu.37) Sr2 Co O5
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              347
_journal_page_last               355
_journal_volume                  156
_journal_year                    1989
_chemical_formula_sum            'Cu O5.24 Sr2 Tl'
_chemical_name_systematic        'Tl Sr2 Cu O5.24'
_space_group_IT_number           123
_symmetry_space_group_name_Hall  '-P 4 2'
_symmetry_space_group_name_H-M   'P 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.7344
_cell_length_b                   3.7344
_cell_length_c                   9.007
_cell_volume                     125.609
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            Kim_JCOMAH_1989_1906.cif
_cod_data_source_block           Cu1O5.24Sr2Tl1
_cod_original_cell_volume        125.6093
_cod_original_formula_sum        'Cu1 O5.24 Sr2 Tl1'
_cod_database_code               1530164
Cation and Oxygen Disorder in the Structures Tl Sr2 Cu O5 And (Pb.63 Cu.37) Sr2 Co O5
Kim, J.S.; Swinnea, J.S.; Steinfink, H.; Journal of the Less-Common Metals 156 (1989) 347–355; doi:

data_1530165
_publ_section_title
;
 Cation and Oxygen Disorder in the Structures Tl Sr2 Cu O5 And (Pb.63
 Cu.37) Sr2 Co O5
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              347
_journal_page_last               355
_journal_volume                  156
_journal_year                    1989
_chemical_formula_sum            'Co Cu0.37 O5 Pb0.63 Sr2'
_chemical_name_systematic        'Pb0.63 Cu0.37 Sr2 Co O5'
_space_group_IT_number           123
_symmetry_space_group_name_Hall  '-P 4 2'
_symmetry_space_group_name_H-M   'P 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.7591
_cell_length_b                   3.7591
_cell_length_c                   8.962
_cell_volume                     126.641
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            Kim_JCOMAH_1989_1907.cif
_cod_data_source_block           Co1Cu0.37O5Pb0.63Sr2
_cod_original_cell_volume        126.6405
_cod_original_formula_sum        'Co1 Cu0.37 O5 Pb0.63 Sr2'
_cod_database_code               1530165
Evidence for near zero coordinate silver(I). the crystal structures of fully and partially hydrated fully Ag+ exchanged zeolite A
Kim, Y.; Seff, K.; Journal of Physical Chemistry 82 (1978) 1071–1077; doi:

data_1530166
_publ_section_title
;
 Evidence for near zero coordinate silver(I). the crystal structures of
 fully and partially hydrated fully Ag+ exchanged zeolite A
;
_journal_name_full               'Journal of Physical Chemistry'
_journal_page_first              1071
_journal_page_last               1077
_journal_volume                  82
_journal_year                    1978
_chemical_formula_sum            'Ag12 Al12 H6 O51 Si12'
_chemical_name_systematic        'Ag12 Si12 Al12 O48 (H2 O)3'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   12.206
_cell_length_b                   12.206
_cell_length_c                   12.206
_cell_volume                     1818.528
_citation_journal_id_ASTM        JPCHAX
_cod_data_source_file            Kim_JPCHAX_1978_445.cif
_cod_data_source_block           H6Ag12Al12O51Si12
_cod_original_cell_volume        1818.529
_cod_original_formula_sum        'H6 Ag12 Al12 O51 Si12'
_cod_database_code               1530166
The homogeneity ranges, order-disorder transition, and structures of the nonstoichiometric monosulfides of zirconium
Kim, S.-J.; Nguyen, T.-H.; Franzen, H.F.; Journal of Solid State Chemistry 70 (1987) 88–92; doi:

data_1530167
_publ_section_title
;
 The homogeneity ranges, order-disorder transition, and structures of the
 nonstoichiometric monosulfides of zirconium
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              88
_journal_page_last               92
_journal_volume                  70
_journal_year                    1987
_chemical_formula_sum            'S Zr0.75'
_chemical_name_systematic        'Zr.75 S'
_space_group_IT_number           166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   3.6295
_cell_length_b                   3.6295
_cell_length_c                   17.885
_cell_volume                     204.039
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Kim_JSSCBI_1987_1477.cif
_cod_data_source_block           S1Zr0.75
_cod_original_formula_sum        'S1 Zr0.75'
_cod_database_code               1530167
Synthesis and Crystal Structure of Na V3 P3 O12: A Stuffed Structure of alpha-Cr P O4
Kinomura, N.; Muto, F.; Kumada, N.; Matsui, N.; Journal of Solid State Chemistry 79 (1989) 232–237; doi:

data_1530168
_publ_section_title
;
 Synthesis and Crystal Structure of Na V3 P3 O12: A Stuffed Structure of
 alpha-Cr P O4
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              232
_journal_page_last               237
_journal_volume                  79
_journal_year                    1989
_chemical_formula_sum            'Na O12 P3 V3'
_chemical_name_systematic        'Na V3 (P3 O12)'
_space_group_IT_number           74
_symmetry_space_group_name_Hall  '-I 2b 2'
_symmetry_space_group_name_H-M   'I m m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   10.488
_cell_length_b                   13.213
_cell_length_c                   6.455
_cell_volume                     894.521
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Kinomura_JSSCBI_1989_1793.cif
_cod_data_source_block           Na1O12P3V3
_cod_original_cell_volume        894.5206
_cod_original_formula_sum        'Na1 O12 P3 V3'
_cod_database_code               1530168
Barium-lanthanide double molybdates Ba Ln2 (Mo O4)4. II. Crystal structure of Ba Nd2 (Mo O4)4
Kiseleva, I.I.; Sirota, M.I.; Ozerov, R.P.; Balakireva, T.P.; Maier, A.A.; Kristallografiya 24 (1979) 1277–1279; doi:

data_1530169
_publ_section_title
;
 Barium-lanthanide double molybdates Ba Ln2 (Mo O4)4. II. Crystal
 structure of Ba Nd2 (Mo O4)4
;
_journal_name_full               Kristallografiya
_journal_page_first              1277
_journal_page_last               1279
_journal_volume                  24
_journal_year                    1979
_chemical_formula_sum            'Ba Mo4 Nd2 O16'
_chemical_name_systematic        'Ba Nd2 (Mo O4)4'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-B 2b'
_symmetry_space_group_name_H-M   'B 1 1 2/b'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                91.05
_cell_formula_units_Z            4
_cell_length_a                   5.329
_cell_length_b                   19.396
_cell_length_c                   12.804
_cell_volume                     1323.216
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Kiseleva_KRISAJ_1979_639.cif
_cod_data_source_block           Ba1Mo4Nd2O16
_cod_original_sg_symbol_Hall     '-C 2yc (-x,z,y)'
_cod_original_formula_sum        'Ba1 Mo4 Nd2 O16'
_cod_database_code               1530169
The crystal structure of K3 Cu (N O2)3
Klanderman, K.A.; Hamilton, W.C.; Bernal, I.; Inorganica Chimica Acta 23 (1977) 117–129; doi:

data_1530170
_publ_section_title
;
 The crystal structure of K3 Cu (N O2)3
;
_journal_name_full               'Inorganica Chimica Acta'
_journal_page_first              117
_journal_page_last               129
_journal_volume                  23
_journal_year                    1977
_chemical_formula_sum            'Cu K3 N5 O10'
_chemical_name_systematic        'K3 Cu (N O2)5'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            16
_cell_length_a                   21.7
_cell_length_b                   18.94
_cell_length_c                   10.88
_cell_volume                     4471.658
_citation_journal_id_ASTM        ICHAA3
_cod_data_source_file            Klanderman_ICHAA3_1977_122.cif
_cod_data_source_block           Cu1K3N5O10
_cod_original_cell_volume        4471.659
_cod_original_sg_symbol_Hall     '-P 2ac 2n (z,x,y)'
_cod_original_formula_sum        'Cu1 K3 N5 O10'
_cod_database_code               1530170
Darstellung und Kristallstruktur von Na5 Co2 S5
Klepp, K.O.; Bronger, W.; Journal of the Less-Common Metals 98 (1984) 165–172; doi:

data_1530171
_publ_section_title
;
 Darstellung und Kristallstruktur von Na5 Co2 S5
;
_journal_name_full               'Journal of the Less-Common Metals'
_journal_page_first              165
_journal_page_last               172
_journal_volume                  98
_journal_year                    1984
_chemical_formula_sum            'Co2 Na5 S5'
_chemical_name_systematic        'Na5 Co2 S5'
_space_group_IT_number           107
_symmetry_space_group_name_Hall  'I 4 -2'
_symmetry_space_group_name_H-M   'I 4 m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.15
_cell_length_b                   9.15
_cell_length_c                   6.222
_cell_volume                     520.921
_citation_journal_id_ASTM        JCOMAH
_cod_data_source_file            Klepp_JCOMAH_1984_958.cif
_cod_data_source_block           Co2Na5S5
_cod_original_cell_volume        520.9214
_cod_database_code               1530171
Thermal stability and synthesis of crystals of double molybdates (K2 R2)(2+) (Mo O4)3 (R = Mg, Ni, Co, or Zn), and crystal structure of beta-K2 Mg2 (Mo O4)3
Klevtsov, P.V.; Klevtsova, R.F.; Kim, V.G.; Kristallografiya 25 (1980) 301–311; doi:

data_1530172
_publ_section_title
;
 Thermal stability and synthesis of crystals of double molybdates (K2
 R2)(2+) (Mo O4)3 (R = Mg, Ni, Co, or Zn), and crystal structure of
 beta-K2 Mg2 (Mo O4)3
;
_journal_name_full               Kristallografiya
_journal_page_first              301
_journal_page_last               311
_journal_volume                  25
_journal_year                    1980
_chemical_formula_sum            'K2 Mg2 Mo3 O12'
_chemical_name_systematic        'K2 Mg2 (Mo O4)3'
_space_group_IT_number           19
_symmetry_space_group_name_Hall  'P 2ac 2ab'
_symmetry_space_group_name_H-M   'P 21 21 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            12
_cell_length_a                   31.775
_cell_length_b                   10.594
_cell_length_c                   10.603
_cell_volume                     3569.228
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Klevtsov_KRISAJ_1980_645.cif
_cod_data_source_block           K2Mg2Mo3O12
_cod_database_code               1530172
The Crystal Hydrooxichloride Y3 Cl2 O (O H)5
Klevtsova, R.F.; Klevtsov, P.V.; Kozeeva, L.P.; Izvestiya Akademii Nauk SSSR, Neorganicheskie Materialy 3 (1967) 1430–1434; doi:

data_1530173
_publ_section_title
;
 The Crystal Hydrooxichloride Y3 Cl2 O (O H)5
;
_journal_name_full
'Izvestiya Akademii Nauk SSSR, Neorganicheskie Materialy'
_journal_page_first              1430
_journal_page_last               1434
_journal_volume                  3
_journal_year                    1967
_chemical_formula_sum            'Cl2 H5 O6 Y3'
_chemical_name_systematic        'Y3 Cl2 O (O H)5'
_space_group_IT_number           59
_symmetry_space_group_name_Hall  '-P 2c 2bc'
_symmetry_space_group_name_H-M   'P n m m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.24
_cell_length_b                   13.23
_cell_length_c                   3.73
_cell_volume                     406.627
_citation_journal_id_ASTM        IVNMAW
_cod_data_source_file            Klevtsova_IVNMAW_1967_1932.cif
_cod_data_source_block           H5Cl2O6Y3
_cod_original_cell_volume        406.6267
_cod_original_sg_symbol_Hall     '-P 2ab 2a (z,x,y)'
_cod_original_formula_sum        'H5 Cl2 O6 Y3'
_cod_database_code               1530173
Crystal structure of the binary molybdates K8 Zr (Mo O4)6 and K8 Hf (Mo O4)6
Klevtsova, R.F.; Glinskaya, L.A.; Pasechnyuk, N.P.; Kristallografiya 22 (1977) 1191–1195; doi:

data_1530174
_publ_section_title
;
 Crystal structure of the binary molybdates K8 Zr (Mo O4)6 and K8 Hf (Mo
 O4)6
;
_journal_name_full               Kristallografiya
_journal_page_first              1191
_journal_page_last               1195
_journal_volume                  22
_journal_year                    1977
_chemical_formula_sum            'K8 Mo6 O24 Zr'
_chemical_name_systematic        'K8 Zr (Mo O4)6'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 119
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   10.2
_cell_length_b                   11.85
_cell_length_c                   13.12
_cell_volume                     1386.985
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Klevtsova_KRISAJ_1977_343.cif
_cod_data_source_block           K8Mo6O24Zr1
_cod_original_cell_volume        1386.984
_cod_original_formula_sum        'K8 Mo6 O24 Zr1'
_cod_database_code               1530174
Crystal structure of the binary molybdates K8 Zr (Mo O4)6 and K8 Hf (Mo O4)6
Klevtsova, R.F.; Glinskaya, L.A.; Pasechnyuk, N.P.; Kristallografiya 22 (1977) 1191–1195; doi:

data_1530175
_publ_section_title
;
 Crystal structure of the binary molybdates K8 Zr (Mo O4)6 and K8 Hf (Mo
 O4)6
;
_journal_name_full               Kristallografiya
_journal_page_first              1191
_journal_page_last               1195
_journal_volume                  22
_journal_year                    1977
_chemical_formula_sum            'Hf K8 Mo6 O24'
_chemical_name_systematic        'K8 Hf (Mo O4)6'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 118.82
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   10.175
_cell_length_b                   11.771
_cell_length_c                   13.102
_cell_volume                     1374.859
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Klevtsova_KRISAJ_1977_344.cif
_cod_data_source_block           Hf1K8Mo6O24
_cod_original_formula_sum        'Hf1 K8 Mo6 O24'
_cod_database_code               1530175
Crystal structure of the double molybdate K2 Ni (Mo O4)2
Klevtsova, R.F.; Klevtsov, P.V.; Kristallografiya 23 (1978) 261–265; doi:

data_1530176
_publ_section_title
;
 Crystal structure of the double molybdate K2 Ni (Mo O4)2
;
_journal_name_full               Kristallografiya
_journal_page_first              261
_journal_page_last               265
_journal_volume                  23
_journal_year                    1978
_chemical_formula_sum            'K2 Mo2 Ni O8'
_chemical_name_systematic        'K2 Ni (Mo O4)2'
_space_group_IT_number           64
_symmetry_space_group_name_Hall  '-C 2ac 2'
_symmetry_space_group_name_H-M   'C m c a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.469
_cell_length_b                   19.035
_cell_length_c                   10.84
_cell_volume                     1747.488
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Klevtsova_KRISAJ_1978_309.cif
_cod_data_source_block           K2Mo2Ni1O8
_cod_original_formula_sum        'K2 Mo2 Ni1 O8'
_cod_database_code               1530176
Crystal structure and polymorphism of potassium-zinc tungstate K4 Zn (W O4)3
Klevtsova, R.F.; Ivannikova, N.V.; Klevtsov, P.V.; Kristallografiya 24 (1979) 257–264; doi:

data_1530177
_publ_section_title
;
 Crystal structure and polymorphism of potassium-zinc tungstate K4 Zn (W
 O4)3
;
_journal_name_full               Kristallografiya
_journal_page_first              257
_journal_page_last               264
_journal_volume                  24
_journal_year                    1979
_chemical_formula_sum            'K4 O12 W3 Zn'
_chemical_name_systematic        'K4 Zn (W O4)3'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                105.55
_cell_angle_beta                 106.16
_cell_angle_gamma                94.13
_cell_formula_units_Z            2
_cell_length_a                   9.957
_cell_length_b                   9.891
_cell_length_c                   7.807
_cell_volume                     702.470
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Klevtsova_KRISAJ_1979_413.cif
_cod_data_source_block           K4O12W3Zn1
_cod_original_cell_volume        702.47
_cod_original_formula_sum        'K4 O12 W3 Zn1'
_cod_database_code               1530177
Triclinic modification of lithium-rare earth tungstates Li Ln (W O4)2, where Ln is La-Sm
Klevtsova, R.F.; Kharchenko, L.Yu.; Borisov, S.V.; Efremov, V.A.; Klevtsov, P.V.; Kristallografiya 24 (1979) 446–454; doi:

data_1530178
_publ_section_title
;
 Triclinic modification of lithium-rare earth tungstates Li Ln (W O4)2,
 where Ln is La-Sm
;
_journal_name_full               Kristallografiya
_journal_page_first              446
_journal_page_last               454
_journal_volume                  24
_journal_year                    1979
_chemical_formula_sum            'Li O8 Pr W2'
_chemical_name_systematic        'Li Pr (W O4)2'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                114.47
_cell_angle_beta                 115.37
_cell_angle_gamma                56.23
_cell_formula_units_Z            2
_cell_length_a                   7.467
_cell_length_b                   8.03
_cell_length_c                   7.089
_cell_volume                     310.369
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Klevtsova_KRISAJ_1979_415.cif
_cod_data_source_block           Li1O8Pr1W2
_cod_original_cell_volume        310.3692
_cod_original_formula_sum        'Li1 O8 Pr1 W2'
_cod_database_code               1530178